Structural Diversity Modulated by the Ratios of a Ternary Solvent Mixture: Syntheses, Structures, and Luminescent Properties of Five Zinc(II) Metal‒Organic Frameworks
Wan, Xiuyan; Jiang, Feilong; Chen, Lian; Wu, Mingyan; Zhang, Mingjian; Pan, Jie; Su, Kongzhao; Yang, Yan; Hong, Maochun; Crystal Growth & Design 15 (2015) 1481–; doi:10.1021/cg501828u

data_4512684
_publ_section_title
;
 Structural Diversity Modulated by the Ratios of a Ternary Solvent
 Mixture: Syntheses, Structures, and Luminescent Properties of Five
 Zinc(II) Metal--Organic Frameworks
;
_journal_issue                   3
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              1481
_journal_paper_doi               10.1021/cg501828u
_journal_volume                  15
_journal_year                    2015
_chemical_formula_sum            'C36 H12 O19 Zn3'
_chemical_formula_weight         944.57
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2013
_cell_angle_alpha                69.517(6)
_cell_angle_beta                 75.565(5)
_cell_angle_gamma                86.284(5)
_cell_formula_units_Z            2
_cell_length_a                   12.4752(7)
_cell_length_b                   15.3763(9)
_cell_length_c                   17.9551(12)
_cell_measurement_reflns_used    7502
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      72.9890
_cell_measurement_theta_min      3.6460
_cell_volume                     3123.6(4)
_computing_cell_refinement       'CrysAlisPro, Agilent Technologies'
_computing_data_collection       'CrysAlisPro, Agilent Technologies'
_computing_data_reduction        'CrysAlisPro, Agilent Technologies'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 10.5594
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.965
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Atlas'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0475
_diffrn_reflns_av_unetI/netI     0.0508
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.965
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            23780
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.965
_diffrn_reflns_theta_full        67.684
_diffrn_reflns_theta_max         73.709
_diffrn_reflns_theta_min         3.069
_exptl_absorpt_coefficient_mu    1.786
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.92487
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'CrysAlisPro, Agilent Technologies'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.004
_exptl_crystal_description       prism
_exptl_crystal_F_000             940
_exptl_crystal_size_max          0.180
_exptl_crystal_size_mid          0.160
_exptl_crystal_size_min          0.150
_platon_squeeze_details
;
;
_refine_diff_density_max         3.237
_refine_diff_density_min         -0.692
_refine_diff_density_rms         0.155
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.011
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     523
_refine_ls_number_reflns         12192
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.011
_refine_ls_R_factor_all          0.1035
_refine_ls_R_factor_gt           0.0918
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.2000P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2509
_refine_ls_wR_factor_ref         0.2650
_reflns_Friedel_coverage         0.000
_reflns_number_gt                9034
_reflns_number_total             12192
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            cg501828u_si_002.cif
_cod_data_source_block           complex3
_cod_depositor_comments
'Adding full bibliography for 4512682--4512686.cif.'
_cod_database_code               4512684
_shelx_estimated_absorpt_t_min   0.739
_shelx_estimated_absorpt_t_max   0.776
_shelxl_version_number           2013-4
_shelx_res_checksum              68594
_shelx_hkl_checksum              35350